Magnetic polarization of noble metals by Co nanoparticles in
-capped granular multilayers
= Cu, Ag, and Au): An x-ray magnetic circular dichroism study
J. Bartolomé,1 L. M. García,1F. Bartolomé,1F. Luis,1R. López-Ruiz,1F. Petroff,2C. Deranlot,2F. Wilhelm,3A. Rogalev,3
P. Bencok,3N. B. Brookes,3L. Ruiz,4and J. M. González-Calbet4
1Instituto de Ciencia de Materiales de Aragón and Departamento de Física de la Materia Condensada, CSIC-Universidad de Zaragoza,
50009 Zaragoza, Spain
2Unité Mixte de Physique CNRS/Thales, Route Départementale 128, 91767 Palaiseau Cedex, France and Université Paris-Sud, 91405
Orsay Cedex, France
3European Synchrotron Radiation Facility, Boite Postale 220, F-38043 Grenoble, France 4Departamento de Química Inorgánica, Universidad Complutense de Madrid, E-28040 Madrid, Spain
共Received 8 November 2007; revised manuscript received 14 March 2008; published 15 May 2008兲
X-ray magnetic circular dichroism spectra have been recorded at theL2,3edges of Co, Cu, Ag, and Au, and at theKedges of Co and Cu for a series of multilayer systems of partially self-assembled Co nanoparticles, both capped with alumina and with different metals共Cu, Ag, and Au兲. The orbital and spin momentsmLand mSand their ratiomL/mS, for Co, Cu, Ag, and Au, have been determined from those measurements. The trend of increasingmL/mS for Co is the same as found for increasing the effective anisotropyKeffalumina ⬍Cu
⬍Ag⬍Au capped. It is shown that the relative increase in the surface contribution for both quantities, 共mL/mS兲surf and KS, is directly correlated. It is argued that the increase in mL with metal capping actually
reflects an increase in the anisotropy of the orbital moment for the Co surface atoms. The redistribution of the number of holes in the noble metal bands by hybridization with the Co surface atom 3d band and the polarization of thend band by exchange interaction with the Co bands give rise to the magnetic moments derived for the three noble metals investigated.
DOI:10.1103/PhysRevB.77.184420 PACS number共s兲: 75.50.Tt, 75.20.⫺g, 75.30.Gw, 73.22.⫺f
Decreasing the size of particles to the nanometric scale leads to a preponderance of the number of surface atoms with respect to the core ones. In many cases, the particles are embedded in a supporting matrix or covered by a shell of different composition. Therefore, the interface atoms of the particle and the environment are expected to play an impor-tant role in the magnetic properties of each individual par-ticle and, hence, of the system formed by the ensemble of particles, surrounding shell and interparticle connecting mat-ter.
A good example of the previous statement is a system consisting of metallic Co nanoparticles with average diam-eter 具D典 in the range of 1–4 nm, embedded in amorphous alumina. The energy barrier hindering the reversal of the magnetic moment is U=KeffV for not-interacting particles,
where Keff is the magnetic anisotropy effective constant. It
has been experimentally shown that Keff inversely depends
where KS is the magnetic surface anisotropy constant.1 For the particles in the aforementioned range of diameters, the surface contribution is dominant. This expression has been empirically accepted as a proof of the dominating effect of surface anisotropy, although a note of attention should be mentioned; in a recent theoretical work, this expression has been found to be fulfilled by Co particles only when there is a certain elongation in the particle shape.2
Another quantity that has been found to depend on the Co particle average diameter is the ratio of orbital moment with
respect to spin moment mL/mS, as determined from x-ray magnetic circular dichroism 共XMCD兲 measurements.3 The Co particles embedded in alumina also show the same in-verse relationship to具D典.4Therefore,KeffandmL/mSseem to be correlated and dependent on the particle size.
In a previous work, it was shown that the interface be-tween the particle and the surrounding matrix could be modi-fied by capping the Co nanoparticles with Cu or Au. The cap completely surrounds each particle, therefore it effectively modifies the matrix in which the particle is embedded. In both cases, Keff increased with respect to the value
for the alumina-capped particles, with the trend KeffAl2O3 ⬍KeffCu⬍KeffAu.5–7Likewise, an increase in the Com
L/mScould be observed for the two capping cases, increasing with the same trend.6,7Varying the matrix seems to have, therefore, a strong impact on Keff.
In this work, the noble metals Cu, Ag, and Au have been used to cap the Co particles, and to modify in this way the matrix in which the particles are embedded, from the insu-lating case of Al2O3to the conducting case of metals, while maintaining all the other parameters. In this way, dipolar interactions may be assumed to contribute to the U by a similar amount, while exchange interactions are too short ranged to modify it.7Therefore, to study the interface effects Co granular multilayers, with the same average diameter
具D典= 3 nm and interparticle distances, have been studied as a function of capping substitution. These metals have nearly filled 3d10, 4d10, and 5d10 bands and are diamagnetic in the
absence of any hybridization.
It is known from studies on Co thin films capped with Cu and Au that the interface plays a paramount role in the modi-fication of the surface anisotropy8and that the noble metals 共Cu, Ag, or Au兲 become polarized by the magnetic Co.9–12
Although the three metals share ad10-type band, thend
spin-orbit coupling differs by a factor of 6 from Cu to Au, and the Fermi energy also markedly differs. Therefore, the interac-tions of thendband electrons with the Co surface atoms can be systematically modified. The same interactions should be effective in the capped Co nanoparticles, so it was deemed interesting to study the resulting variations of the particle magnetic properties to gain information on the mechanism giving rise to an enhancement of the anisotropy. Because of the element selectivity and high sensitivity of the present XMCD setups, this technique has been applied to obtain in-formation on the orbital and spin moment components of the Co and the capping metals independently.
The samples are prepared by sequential sputtering on a Si substrate of amorphous alumina buffer layer, Co, and the capping material, either alumina, Cu, Ag, or Au. The forma-tion of Co aggregates on the amorphous alumina is the result of three-dimensional growth because of the different surface energies between alumina and Co. The metal and alumina are deposited using Ar plasma at a radio frequency power of 100 W. The substrate temperature is kept constant at 293 K and the Ar pressure is 4⫻10−3 Torr. Co aggregates are formed with 具D典, which linearly depends on the nominal thicknesstCo that the layer would have if it was continuous,
i.e., on the Co deposition time. 具D典 can be changed in the range 0.7⬍具D典⬍5 nm with a guarantee that the particles do not touch one another.13,14 The alumina or metal capping layer deposited on the so formed particles completely sur-rounds each particle 共see below兲, therefore it can be envis-aged as a matrix in which the particle is embedded. It is described by its nominal thicknesstM. On top of the capping layer, a new alumina layer is deposited to act subsequently as generator of the new layer of Co particles. It is interesting to note that, at least for some of the thicknesses, the new par-ticles predominantly form in the valleys created by the pre-vious granular layer.15 The process may continue until the desired number of trilayers N is obtained, which was N
⬇20 in the present samples for XMCD experiments. The samples consisted of platelets of 1⫻1 cm2.
The transmission electron microscopy 共TEM兲 study was carried out with a JEOL 3000FEG electron microscope fitted with an Oxford LINK electron dispersive spectrometry ana-lyzer. Cross-sectional TEM specimens were prepared by glu-ing two films face to face, followed by slicglu-ing, grindglu-ing, polishing, and dimpling. Special care was taken to avoid irradiation damage during ion milling by working at a low angle 共7°兲 and a low voltage 共3.5 kV兲 and by cooling the sample using liquid nitrogen.
The x-ray absortion spectroscopy 共XAS兲and XMCD ex-periments have been performed at the European Synchrotron Radiation Facility 共ESRF兲in Grenoble at the ID08共Cu and CoL2,3edges兲and at the ID12共Co and CuKedges, and Ag
and AuL2,3 edges兲 beamlines. At the ID08 beamline, an
APPLE-II undulator and a spherical grating monochromator were used. The degree of polarization was⬃100%. The total electron yield detection method was employed. The beam
direction, parallel to the applied magnetic field, had an inci-dent angle of 15° with respect to the normal to the plate.
At the ID12 beamline, the undulators APPLE-II and He-lios II were employed, and a double-Si共111兲-crystal mono-chromator provided a monochromatized beam. The polariza-tion was over 90% in all cases, except at the energies of the AgL2andL3edges where it was 36% and 24%, respectively.
The detection technique used in the ID12 experiments was fluorescence in backscattering geometry. The XMCD signal was obtained by a direct difference of the XAS spectra re-corded with opposite helicities at each fixed magnetic field value for both orientations of the field. The applied field was 1 T and the temperature was T= 5 K in all cases. The field was applied with an incident angle of 75° with respect to the normal to the plate. The data shown for Ag and Au are the average of several tens of independent measurements
The coercive field extracted from magnetic hysteresis data at any temperature is isotropic. Therefore, there is no evi-dence of the capping inducing any preferred orientation for the anisotropy axis. This supports our assumption that the particles can be described well in terms of an average diam-eter 具D典. The effective magnetic average diameter is deter-mined from the analysis of the magnetizationM共H兲, fitting it to the Langevin function for a particle with diameter D, av-eraged over a Gaussian distribution of D, and the suscepti-bility 共T兲 for Curie–Weiss behavior averaged in the same way. The procedure has been extensively described in Ref.1. Once the magnetic average diameter has been determined, a scaling analysis of the out-of-phase susceptibility
⬙yields the distribution of activation energiesUfor a given sample. Then, knowing the distributions ofDandU, one accurately derives Keff= 6U共具D典兲/共具D典3兲.1,7
The samples which were measured had an average Co particle diameter of 具D典= 3 nm, except in the case of Au capping in which a sample with具D典= 1.8 nm was also mea-sured. The XAS spectra at the CoL3edge of all the samples reported 关see Fig. 5共a兲, as an example兴are characteristic of metallic Co; i.e., we do not observe any prepeak, or shoulder above the peak, distinctive of the presence of Co-O bonds.16 Therefore, we are quite sure that the Co particles are not oxidized during the fabrication process.
III. MORPHOLOGICAL AND STRUCTURAL CHARACTERIZATION
The morphological and structural characteristics of the Co particles, which are embedded in alumina, had been previ-ously studied in detail by TEM, extended x-ray absortion fine structure, and x-ray diffraction.13–17 It has been shown14,18 that Co particles with 具D典⬍3 nm 共tCo⬍0.8 nm兲, as is the
present case, crystallize in the fcc phase, while fortCohigher
difference between the nominal Co deposition and a direct count of Co clusters from plane view TEM, resulting in Co/Al2O3 samples that are xpara= 77% and 45% for the
tCo= 0.4 and 0.7 nm samples, respectively. Indirectly, xpara has been deduced from M共H兲 measurements, yielding the values xpara= 50% and 25% for the tCo= 0.4 andtCo= 0.7 nm
samples, respectively.13,19 Note that these values somewhat differ from the more direct results obtained from the TEM measurements for Co/Al2O3samples.
To assess the morphology and number of layers of the films, a TEM study has been performed on cross sections of the Cu-, Ag-, and Au-capped multilayers, with nominal thicknesses tCo= 0.7 nm, tM= 1.5 nm, and tAl2O3= 3 nm. In
Fig. 1共a兲, the image of the Si/Al2O3/共Co/Cu/Al2O3兲 ⫻15/Al2O3 sample shows an ordered arrangement of 15
dark and bright fringes of 4 and 1.2 nm average thicknesses, respectively, which perfectly agrees with the nominal se-quential layer deposition in the system. A similar dark 共3.5 nm兲 and bright 共2.5 nm兲 fringe distribution is observed for the Si/Al2O3/共Co/Au/Al2O3兲⫻25/Al2O3 system where 25 layers are evident关Fig.1共c兲兴. In both cases, the dark fringes are apparently built up of particles with different sizes and shapes with a clear tendency of elongation. In contrast to the cases of Co/Cu and Co/Au, the fringes are not so well de-fined for Co/Ag. While keeping a general layered aspect, they are more randomly distributed 关Fig. 1共b兲兴 than in the other samples. In spite of this more disordered arrangement, the clusters are well detached from one another.关Fig.2共b兲兴. The average diameter of the particles ranges between 3 and 5 nm.
In order to get more structural information, a high reso-lution transmission electron microscopy共HRTEM兲study was done. In all three cases, HRTEM images 关Figs. 2共a兲–2共c兲兴 reveal the crystalline nature of the particles, within the dark fringes for Co/Cu and Co/Au, and the dark particles in Co/ Ag, while they show the amorphous character of the bright fringes. The elongated shapes inferred at low magnification can be understood as a consequence of the particles superpo-sition along a row. This can be better observed in Fig. 2共a兲 corresponding to the external layer of the Co/Au film where the particle concentration decreases.
The analysis of the chemical composition by means of EDX analysis indicates the coexistence of the two elements in the Co/Cu, Co/Ag, and Co/Au samples. However, the spot resolution is not sufficient to resolve the localization of Co and the metal. In some particles, a light gray aura seems to surround the darker gray core, while inside the Co/Cu layers, near the thinner border of the TEM sample, a lighter gray band connects the darker particle spots. Both lighter gray bands could be indicative of the noble metal surrounding the Co particle. Figures3共a兲–3共c兲are magnified HRTEM images of individual particles of the Cu, Ag, and Au samples, re-spectively, and include the corresponding fast Fourier trans-form 共FFT兲. In all of the three cases, the measured period-icities in the images as well as the distances and angles on the FFT are in agreement with a fcc lattice along关101¯兴zone axis. The splitting of the spots in some cases indicates the
20 nm 20 nm
FIG. 1. TEM cross sections of granular
multilayers with tCo= 0.7 nm, tM= 1.5 nm, and tAl2O3= 3 nm. 共a兲 Si/Al2O3/共Co/Cu/Al2O3兲⫻15/Al2O3, 共b兲 Si/Al2O3/共Co/Ag/Al2O3兲⫻20/Al2O3, and 共c兲 Si/Al2O3/共Co/Au/Al2O3兲⫻25/Al2O3. The dark spots correspond to the Co particles covered by the noble metal. The intermediate light area is the amorphous Al2O3.
presence of twinning in the particle 关Fig. 3共c兲兴. This can indeed also be observed in those particles where two orien-tations are evident. On the other hand, there is no clear evi-dence of a formation of a new intermetallic compound.
The overall picture in the three studied samples is that the Co particles are surrounded by the capping layer that acts like a matrix, completely covering the particles. The regular-ity found in the alumina-capped sample, i.e., with alumina as a matrix, is less clear in these samples. However, most of the particles seem to be detached from one another or connected within the layer by the noble metal. From the HRTEM, it was not possible to discern the interface between the Co particle and the capping metal because of the common fcc structure and the similarity in interatomic distances. The par-ticles are not spherical, but irregular. In view of the HRTEM images in Fig.3, where the crystallinity of the Co core
par-ticles is evidenced, the possibility that the parpar-ticles are fac-eted is large.
Magnetic measurements performed on the tCo= 0.7 nm samples enabled us to determine their blocking temperatures TB. These data for Co/Al2O3, Co/Cu, and Co/Au were given
elsewhere.6In this paper, data for the Co/Ag samples are first reported, and it is nice to verify that the trend followed is that of alumina⬍Cu⬍Ag⬍Au capped共see TableI兲. Moreover, Kefffor the four systems also follows the same trend in
in-creasing values. The surface anisotropyKSdeduced from the experimental results after applying Eq. 共1兲 with具D典= 3 nm are included in TableI. The increase in anisotropy with cap-ping and a decrease in average diameter, as described in Ref. 6 for the Co/Al2O3, Co/Cu, and Co/Au cases, are also
veri-fied by Co/Ag, being intermediate with respect to Co/Cu and Co/Au, as could be expected from electronic considerations
IV. X-RAY MAGNETIC CIRCULAR DICHROISM IN CAPPED SAMPLES
The XMCD technique may give some direct evidence on the hybridization of the interatomic 3d-nd and the Co intra-atomic 3d-4p bands. In this section, the results on the CoK and Co, Cu, Ag, and AuL2,3 edges are presented for the
alumina-capped and the three metal-capped samples. From a XMCD experiment at the L2,3edges of Co, Cu,
Ag, or Au, one obtains, through the sum rules,20,21 the spin and orbital moments averaged over the core and the surface of the particle and the number of holes nhin the empty ex-change split nd subbands. The sum rules have been applied to the spectra to derive the orbital, spin, and total magnetic moments, and the symbols and sign criteria defined in Ref. 22 have been used below. The constant C=共IL2+IL3兲/nh, where IL2+IL3 are the white-line integrated intensities after subtraction of the contributions from transitions to the con-tinuum, andnh, depend on the normalization method used for the XAS spectra. Therefore, in this paper, all the experimen-tal data show not only the XAS but also the normalized data, and the values of C are explicitly given. For the sake of comparison, we have adopted the normalization procedure for each metal as that found in literature. It was not possible to derive the integrated XAS white-line intensity from our measurements, since the difference in the XAS spectra of the present samples with that of the corresponding bulk metal is inappreciable. Therefore, to obtain the magnetic moments, the method first proposed in Ref. 9has been employed.
It is noteworthy that in the present case of particles, with their anisotropy axes oriented at random, the dipolar termmD cancels out so that the sum rule 共A− 2B兲= −CmS/B yields the spin component mS.AandB are the integrated areas of the L3 andL2 XMCD peaks, respectively. In Figs. 7–9, the
parameters p=A andq=A+B have been depicted. Besides, mL/mS is directly derived from the ratio of the sum rules, which is independent ofnhand of the normalization method used.
To systematize the discussion, the results obtained for one particle size, namely,具D典⬇3 nm, are compared unless oth-erwise explicitly stated. In the experiments, a magnetic field
of 1 T is applied, which is sufficient to saturate the particle spin magnetization, but the paramagnetic moment contribu-tion from xparais negligible.
Under an applied field that saturates the particle magneti-zation共Hⱖ1 T兲, the surface Co spin moment, which is iso-tropic, easily orients along the field, but the surface orbital moment gradually tilts from the direction normal to the par-ticle surface to the direction of the applied field. The mag-netic anisotropy energy associated with spin-orbit coupling is about 2 orders of magnitude larger than the dipole interac-tion, but the crystalline anisotropy is of the order of the s.o. coupling, so the spin and orbital moments are not parallel except when the field is parallel to the local easy axis of magnetization.22The projection of the orbital moment along the applied field directionmL, which is averaged over all the surface of the particle, yields the mean orbital moment in the field direction. Therefore, the contribution of the orbital mo-ment to the XMCD signal is the averaged projection of the local moments in the direction of the applied field共parallel to the photon beam direction in the experiments兲. If the particle is approximated to a sphere, the averaged orbital moment is
mL= 1 3共mL
⬜+ 2m L
where mL⬜ is the orbital contribution normal to the particle surface and mL储 is parallel to it. In the case of other particle shapes, the proportions of mL
tomL⬜may be different.
A. X-ray magnetic circular dichroism at the CoKedge
The XMCD measurements at the CoK edge yield the magnetic moment of the 4pband共hybridizedspconduction
bands兲. In Fig. 4, the collected spectra of the XMCD peaks are shown. The shape and amplitude of the measured peaks are similar to those of metallic Co.10,23 The nonzero signal reflects the spin-dependent polarization caused by the ex-change polarized 3dband by intraatomic hybridization. The sign of the XMCD spectra at the CoKedge is the same as in Ref. 10, where the Co/Cu multilayer has been studied in detail. This result indicates that the coupling between 4pand 3d levels of Co is antiferromagnetic.
TABLE I. Blocking temperatureTB, effective volume anisotropy constantKeff, surface anisotropy con-stantKSobtained fromKeffwith Eq.共1兲, andD= 3 nm, which is determined from magnetic measurements. mL, mS, and mL/mS for the Co and noble metal atoms indicated in the left column, as determined from XMCD measurements. For the fcc bulk Co,mL/mS= 0.078共Ref.27兲, and for all Co,mS= 1.62B共Ref.25兲.
Al2O3cap Cu cap Ag cap Au cap
TB共K兲 30.1共1兲a 35.0共1兲a 37.0 43.0共1兲a
Keff共104 J/m3兲 53.共5兲a 78.共10兲a 110.共6兲 139.共7兲a KS共10−5 J/m2兲 23.2共2兲 35.8共3兲 51.5共4兲 66.0共5兲
mL/mS 0.129共10兲a 0.156共20兲a 0.163共10兲 0.197共10兲a
mL共B兲 0.209共16兲 0.253共30兲 0.264共16兲 0.319共16兲
共mL/mS兲surf 0.224共20兲 0.301共30兲 0.321共20兲 0.419共30兲
m共B兲 −0.087共4兲 −0.072共4兲b −0.078共4兲 −0.072共4兲
mLnd/mSnd 0.32共3兲 0.045共5兲 0.10共5兲a
mLnd共B兲 10共3兲⫻10−4 7共1兲⫻10−4 1.5共5兲⫻10−3
mSnd共B兲 0.010共3兲 0.014共3兲 0.015共1兲
mnd共B兲 0.011共3兲 0.015共3兲 0.016共1兲
-20 0 20 40 60 80
Au Ag Cu
Relative photon energy (eV)
From the comparison of the amplitudes of the XMCD CoK-edge spectra, it was derived that the Co moment in the alumina-capped Co particle is about 20% larger than the one found for the three Co-capped ones. This implies that the number of electrons in the Co 4p band is reduced through contact with the capping metals; i.e., there is hybridization, and on average, it gives rise to a redistribution of electrons at the surface Co atoms. Thexparafraction of the Co atoms does
not contribute to the XMCD signal in a significant way.
B. X-ray magnetic circular dichroism at the CoL2,3
The experimental XMCD spectra at the CoL2,3edges for the alumina-, Cu-, Ag-, and Au-capped Co particles are de-picted in Fig.5, together with one example of XAS, for the sake normalization. The XMCD data normalized to the XMCD L2 peak are shown to highlight the increasing trend
of theL3peak intensity, which, in turn, reflects the increase in mL/mS with the capping of Cu, Ag, and Au. The ratios derived from the measurements for the alumina-, Cu-, Ag-,
and Au-capped samples have values that span from 0.129 for the alumina-capped to 0.197 for the Au-capped Co particles, as shown in TableI.
In Fig. 6,Keffvalues are shown together with the values
ofmL/mSfor samples with the sametCo= 0.7 nm, finding an
excellent linear correlation between these two quantities. The extrapolation of this line nicely gives the measuredKeffand
mL/mSfor the bulk fcc Co.24–26This result clearly indicates that the orbital moment and magnetic anisotropy are related to the capped particles; i.e., the modification of the Co aver-age orbital moment due to the interfacial interactions gives rise to an increase in the average effective anisotropy of the particle. Previously, a linear dependence betweenmL/mSand
Keffwas found for particles differing just on the average size in Co particles deposited on Pt 共Ref. 3兲and in the Co par-ticles embedded in alumina.4Just as for Co thin films,8the correlation between Keff and mL/mS seems to be a general rule in nanoparticles.
At any rate, the enhancement ofmL/mSis larger in nano-particles than in thin films. For example, a maximum value of mL/mS= 0.12 was found for about 5 monolayers of Co deposited on Cu共Ref.27兲; the same value, as maximum, was found in the case of four Co atomic layers in a stair case layer of Co sandwiched between Au.8 The same value was found again in islands of two Co monolayer thickness depos-ited on Au.28
Although the integrated areasIL2+IL3of the alumina- and metal-capped samples should yield direct information onnh for the Co 3d band, we found that experimental errors pre-vent determining coherent results. Therefore, we have ad-hered to the assumption thatnhdepends on the element, and taken the calculated value for bulk Co,nh= 2.49.9The corre-sponding scaling constant for Co, deduced from IL2+IL3 = 15.1共5兲 is C= 60共2兲B−1. Similar nh values have been ob-tained from calculations for small Co clusters 共nh= 2.40兲 共Ref.3兲or in Pt/Co multilayers共nh= 2.45兲.29The approxima-tion that the value ofmS may be considered as varying little from the bulk value, mS= 1.62B 共Ref. 25兲is applied in the rest of the paper. We find a justification to this approximation FIG. 5. 共Color online兲 CoL2,3-edge spectra of the same
sam-ples measured at T= 5 K, 0H= 1 T and incident angle 15°. 共a兲 XAS spectra with positive helicity of the incoming beam 共¯·兲, negative helicity共- - -兲, and mean curve共—兲. The two-step function used is also indicated共–兲.共b兲XMCD spectra normalized to a com-mon L2 peak intensity, 关共blue 쎲兲 Co/Al2O3兴 关共red⌬兲 Co/Cu兴, 关共green쎲兲 Co/Ag兴, and 关共yellow⽧兲 Co/Au兴, for particles with the sametCo= 0.7 nm. Inset: expanded view of theL3peak minima. Note the increase in L3 dichroic intensity in the trend alumina
4 J/m 3 )
in the fact that the average total moment of the Co atoms in the particles, as deduced fromM共H兲measurements, is nearly that of the bulk, irrespective of capping or具D典.6
Since XMCD is probing Co in clusters of similar average diameter, the number of surface and core Co atoms is the same in all four samples. Therefore, the increase in mL/mS with respect to the bulk as a function of capping exclusively reflects an increase due to the surface Co atoms. In the analy-sis of Keff, the separation between surface and core atom
contributions has been successfully applied to understand the enhancement of the surface anisotropy by capping.6A simple core shell model allows us to estimate the fraction of surface atoms with the formula f= 1 −共1 − 0.4/D兲3, with D 共nm兲 共f
= 0.35 for D= 3 nm兲 in the approximation of spherical fcc particles.6Within this model,K
eff=Kbulk共1 −f兲+Ksurff, where
Ksurf refers to the surface atoms, is approximately Keff
=Kbulk+ 6KS/D to within 10% atD= 3 nm.
If we apply the same core shell model to the contributions to mL/mS, the contribution from surface atoms 共mL/mS兲surf may be deduced from the equation
where mL/mS is the measured value averaged over the Co mass forming the particles and共mL/mS兲bulk= 0.078共1兲for fcc Co.27 The resulting values for 共m
L/mS兲surf have been in-cluded in Table I. The values that were found range from 0.224 for Co/Al2O3 to 0.419 for Co/Au; i.e., in the extreme
case of Co/Au, the orbital moments at the surface atoms increase by a factor of 5 with respect to bulk fcc Co.
A highly enhanced orbital magnetism on Co cluster sur-faces in a Cu matrix has been reported earlier.30 These au-thors measured the CoL2,3edges and used a core shell model
to deduce the surface orbital moment from their data, finding a value of mL/mS= 0.35 at the Co surface monolayer, which is in good agreement with our result. Co particles supported on Au have also been measured, although of island or disk-like shape, showing also a large increase inmL/mS with re-spect to the bulk value.31
The XAS branching ratio, which is defined as the ratio of intensities, IL3/共IL2+IL3兲 has been found not to depend on capping and has the value of 0.74共1兲. Since the branching ratio gives a measure of the angular part of the spin-orbit operator, it can be considered that this quantity remains un-altered by capping.32
C. X-ray magnetic circular dichroism at theL2,3edges of the
The capping metals Cu, Ag, and Au have 3d10, 4d10, and 5d10bands, respectively. In the metallic state, as is our case, the bands are not completely filled, and, therefore, yield to a small but distinguishable white line in the XAS experiments. These metals are diamagnetic in the absence of hybridization with other elements and, therefore, give no XMCD signal. However, when in contact with other metals, in particular, ferromagnetic Co, hybridization between the conduction bands alters their number of holes, on one hand, and polar-izes by exchange interaction those bands giving rise to the
splitting into majority up 共completely filled兲 and minority down共partially filled兲spin statesdbands, on the other hand. Then, in the first approximation, the magnetic moment is equal to the average number of electrons removed from the atom, i.e., the number of holesnh. The changes in the occu-pation of the electronic orbitals give rise to a small but mea-surable induced magnetic moment in the capping metal layer. These effects have been found in Co thin films capped with Cu,9Ag,11and Au,12so the three noble metals are polarized by magnetic Co at the Co/M interfaces.
To check whether this also holds for the Co granular capped samples, XMCD experiments at theL2,3edges of Cu,
Ag, and Au have been performed. The measurements were done atT= 7 K, an applied field of0H= 1 T, and an
inci-dence angle of 75°. Indeed, Cu, Ag, and Au show nonzero XMCD signals, indicating that a fraction of the capping at-oms become polarized by the exchange spin polarization with the Co moments 共see Figs.7–9兲.
For the XMCD analysis, we depict the areas subtended by the L3 and L2 peaks, as obtained from direct integration of the data. In the case of Cu,phas been taken at the energy of the minimum of the XAS spectra between the L3 and L2
peaks and q when the integral converges to a constant. For the Ag and Au cases, where the statistical scatter is larger, we give the integration of a smooth Lorentzian function as guide for the eyes, which fits the data for these two metal cappings,
920 930 940 950 960 970 0.0
0.2 0.4 0.6 0.8 1.0 1.2
Cu-L2,3 5K, 1T
920 930 940 950 960 970
-0.020 -0.015 -0.010 -0.005 0.000 0.005 0.010
Photon Energy (eV)
Cu-L2,3 5K, 1 T
-0.04 -0.02 0.00 0.02
as shown in Fig. 8共b兲 for Ag and Fig. 9共b兲 for Au. The energies at whichpandqhave been taken are also shown in Figs.8共bottom兲and9共bottom兲. The error in the integration is considered to be the width of its deviation with respect to the mean guideline and amounts to 15% and 10% in the Ag and Au cases, respectively.
The ratiomL3d/mS3dis directly obtained from the sum rules and is independent of any choice in the scaling constant. For Cu,mL3
= 0.32共3兲, which is larger than the ratio found in other Co granular alloys in the presence of Cu 关mL
= 0.018 共Ref. 33兲兴 and in a random Co90Cu10 alloy 关mL3d/mS3d= 0.09 共Ref. 9兲兴. However, the factors between nh and the white-line area, given in Ref.9, are C= 5.6B
and 14B−1for the mS3d andmL3dsum rules, respectively共 normal-ization of the total L2 and L3 XAS to 1兲, which yield to
= 0.010共3兲BandmL3 d
B. If this method is employed, the value for the ratiomL
= 0.10共3兲, which is quite low but comparable to other determinations. At any rate, the total momentm3d= 0.011共3兲
Bis deduced, while the orbital moment is very small and practically negligible. It is concluded without ambiguity that the Cu-capping layer is magnetically polarized by the Co particles. It is interesting to note that this value is in the range of the predicted polariza-tion per Cu atom adjacent to a Co nanoparticle.34
In the case of the Ag-capped Co particles, a nonzero XMCD at the L2,3edges is observable共Fig.8兲, although the
signal is very small; the larger L3 peak amounting to just a
few per thousand of the XAS signal. Only the high quality of
the ID12 beamline at the ESRF has allowed this experiment. The corrected data are shown in Fig. 8. The ratiomL
= 0.045共5兲is extremely small, as compared to Cu共or Au, see later兲. Therefore, the detected nonzero induced magnetiza-tion can essentially be assigned to the spin component. The determination of the constant C was derived in Ref. 11 by obtaining the white-line excess area with respect to Ag,
⌬Awl, on one hand, and using the method described for the
interpretation of the XAS data35to determine the increase in the number of holes in the sample 共NiFe/Ag multilayers兲
⌬nh, with respect to a pure Ag sample, on the other. Then, finding the quotient C=⌬Awl/⌬nh= 2.3共2兲B−1. The value
= 0.014共3兲Bis obtained, which is higher than that in Cu. This value can only be compared to m4d= 0.0135
B deter-mined for Ag in Ni81Fe19/Ag multilayers.11 The value of
= 7⫻10−4B may be considered as negligible.
The XMCD data at the AuL2,3 edges performed on the
Au-capped Co nanoparticles also indicated that there is a nonzero magnetic moment induced by the hybridization with Co 共Fig. 9兲. The obtained value is mL
= 0.10共5兲. This result is in reasonable agreement with the published value of mL
= 0.12,12where the valueC= 7.8B −1
was used to de-termine mL5
and mS5 d
of Au in a Co12/Au4 multilayer. To
derive C, the values ofIL2 andIL3 were experimentally de-termined from the white line of a reference Au4Mn
com-pound共XAS normalization ofL3edge to 1 and ofL2edge to 0.45兲with respect to the bulk Au XAS signal andnhfrom the difference in the calculated nh values for Au4Mn and bulk
FIG. 8. 共Color online兲Normalized AgL2,3-edge XAS共top兲and XMCD共bottom兲spectra of Si/Al2O3/共Co/Ag/Al2O3兲⫻20/Al2O3. 共-兲Fit to the Lorentzian function.共䊏兲Area integral;共--兲area inte-gral of the Lorentzian. The arrows indicate the higher limit of thep andqintegrals.
Au. Using that constant, mS5d= 0.015共1兲B and mL 5d
⫻10−3B, yielding to a total ofm5d= 0.016共1兲B.
The three capping noble metals are, therefore, polarized by the Co magnetic moments. The negative sign of the L3
peak and the positive sign of theL2one, which are the same
as theL2,3peaks of Co on the same sample, temperature, and
field, indicate that the coupling between the Co average mo-ment and the momo-ment induced in the noble metal is ferro-magnetic. The same sign for this coupling had been found for Co thin films with Cu, Ag, or Au interfaces.9,11,12
The ratio mL/mS is free of any scaling procedure. It is directly deduced from the XMCD signal, therefore it only gives information on those M atoms that are magnetically polarized, i.e., those affected by the exchange field of the magnetic Co. TheM atoms outside of the sphere of influence of Co are silent to the XMCD, although they give a contri-bution to the XAS signal that may hamper the correct deter-mination of the scaling factor C 共see below兲. The fact that the ratiomL
in the three cases studied here have values similar to those found in other cases of the same M in con-tact with Co indicates that this is directly related to the de-gree of hybridization of the 3d of Co with the nd electron band of M at the interface. Thus, it is an intrinsic property related to the two metals involved at the interface.
Besides, the only case in which the presence of an in-duced orbital moment in the capping metal is unambiguously proven is the Au-capped sample. The spin-orbit coupling constants ared= 60, 97, 272, and 608 meV for Co, Cu, Ag, and Au, respectively,36 so the larger m
induced in Au is probably associated with this larger s.o. coupling with re-spect to the other metals.
Another nice result is that mndincreases in the trend Cu, Ag, and Au cappings. This may be related to two mecha-nisms, an increasing number of holes in the nd and nsp bands of the noble metal, since they may also play a role in the hybridization with the 3d band of Co, or an increased exchange polarization of those bands. Each may give rise to the presence of induced moment, independently, although most probably both mechanisms are acting together in this case. Unluckily, the possible variation of nh could not be derived from the direct detection of an increased white line in theseM-capped Co particles with respect to the bulk cor-responding M noble metal, since the error bar in our XAS data does not support this analysis.
In the case of Au capping, the AuL2,3-edge experiments
were also performed on a sample with a smaller diameter,
具D典= 1.8 nm, corresponding to tCo= 0.4 nm. The XMCD
signals are smaller than those for tCo= 0.7 nm and 具D典 = 3 nm. Since the XMCD spectra in both cases are scaled to the L2,3-edge XAS spectra and the XAS spectra for the two
samples are indistinguishable, this implies that the relative number of Au atoms influenced by the Co exchange field is smaller in the case of the sample with smaller Co particles. From the analysis of the AuL2,3XMCD data共Fig.10兲, it is
found thatmL5 d/
is identical fortCo= 0.4 and 0.7 nm, while
the total magnetizations per Au atom are m= 0.005B and 0.017B, respectively, that is, they differ markedly, being
tCo=0.4/mtCo=0.7⬇0.32 the ratio of polarized Au atoms
in one sample with respect to the other. This result is unex-pected, since the number of Co surface atoms which polarize
Au, with respect to the number of core Co atoms, is larger for the particles with smaller diameter. One needs to recollect that those Au atoms in contact with the paramagnetic fraction of the deposited Co are XMCD silent. Therefore, the number of polarized Au atoms is directly related only to the number of Co atoms at the surface of the particles. It is known that the polarization of the noble metal rapidly decays with dis-tance from the interface,9,11being the first shell, and the one sustaining most of the polarized moment. Therefore, the sim-plification that
is done. Here, the nCosurf per unit area of the sample platelet may be estimated from the amount of nominal Co sputtered tCo, the fraction of that Co which forms the particles 共1
−xpara兲, and f as the fraction of the Co atoms in the particle that are located at the surface,
nCosurf=tCo共1 −xpara兲f. 共5兲
The ratio of nAupolarizedfor the two particle sizes is
rAu= tCo共1 −xpara兲ftCo=0.4 tCo共1 −xpara兲ftCo=0.7= 0.86
共1 −xpara兲tCo=0.4 共1 −xpara兲tCo=0.7
The parameter xpara has been determined for both samples
from TEM measurements;13 i.e., for t
Co= 0.4 nm sample,
xpara= 77%, and fortCo = 0.7 nm samplexpara= 45%,
yield-ing the ratio rAu= 0.35, which is in good agreement with the
Thus, the strong reduction inrAumay be explained as due,
essentially, to the different amounts ofxpara existent in each sample and not due to size effects associated with electronic confinement or depth dependent Co moments.
D. X-ray magnetic circular dichroism at the CuKedge
With respect to the K edge of the three capping layer metals, only the XMCD at the CuK edge could be measured.5Since this XMCD nonzero signal probes the 4p holes in the conduction band, this result indicates that the 4p states are hybridized with the Co 3d band holes, via ex-change spin polarization, and become polarized antiparallel to the 3dmoments. On the other hand, its sign is the same as that of the CoK-edge XMCD peak, indicating that the Cu 4p
11880 11920 13720 13760 13800
-0.008 -0.004 0.000 0.004
tCo=0.4 nm tCo=0.7 nm
Photon Energy (eV)
holes are ferromagnetically coupled to the Co 4sp conduc-tion band holes. The mean 4p moment value found was m4p= −0.016共2兲
B, antiparallel to the Co 3d moment and, therefore, parallel to the Co 4p moment.5
The results shown in Sec. I and IV indicate that the elec-tronic structure of the Co atoms at the Co/M interface gov-erns the particle magnetic properties. Indeed, an increasing Keffand, correspondingly,KSare found in the trend alumina, Cu, Ag, and Au caps. On the other hand, a simple evaluation of the orders of magnitude of the anisotropies involved, mag-netocrystalline, shape, or stress, supports the fact that none of them can explain the observed increase in Keff with re-spect to the bulk value, even in the case that the particles were needle shaped.7
As a rough approximation, the Co particles in the M-capped samples have been considered as spheres of aver-age diameter 具D典. However, HRTEM pictures show that the particles are not spherical but irregular, and it can be conjec-tured from the well oriented crystal lattice in the core that the particles are probably faceted. In fact, recent calculations of the anisotropy energy in Co faceted, nonregular polyhedra have given Keffvalues in good agreement with our data for
the alumina-capped particles.37The Co/Minterface probably consists of planar facets of limited dimensions. Therefore, as a guidance, it is reasonable to pay attention to the electronic modifications of Co at the surface of planar Co/M thin films, implicitly two dimensional, for which there exist theoretical and experimental results as to how the Co surface anisotropy is modified by the interfacial metal.
Several calculations of the Co thin film interface aniso-tropy energy have been performed. A freestanding Co mono-layer is predicted to have parallel anisotropy, i.e., negative magnetic anisotropy energy 共MAE兲,38 but capping with Cu, or with 1 monolayer of Au increases the MAE; i.e., it ap-proaches zero, but the anisotropy remains planar.39,40 How-ever, in a Cu/Co/Cu sandwich, i.e., with another Cu capping layer, a positive shift of the anisotropy to nearly zero or even weakly positive MAE38is induced. Moreover, capping with more than 2 monolayers of Au changes the Co anisotropy to perpendicular.40 According to the approach in Ref. 38, the trend of the positive shift in the MAE should be increasing as Co/Cu, Co/Ag, and Co/Au. However, the predicted MAE for Co/Cu and Co/Ag is negative and a conflicting theoretical result states that the MAE in Cu/Co/M-capped sandwiches favors perpendicular anisotropy for M= Cu and Ag, while favors basal for Au.41
The MAE crossover from negative to positive as a func-tion of thickness and Au capping has been nicely explained in terms of the following simple model.42 At the interface, the Co atoms are bonded with one another by the same in-teractions as in the bulk, on one side, while the Co-M inter-actions are evidently different on the other. The case of 3d in-plane and out-of-plane bands is then separately consid-ered. In agreement with the above in-plane and out-of-plane band models, the in-plane band remains identical to the bulk, while the out-of-plane band is modified, giving rise to the
surface anisotropy. It was shown that the MAE depends on the in-plane and out-of-plane 3d bandwidths. This is so be-cause the Co orbital moment mainly arises from the minority band since the majority band has no net orbital moment and the average bandwidth determines the average separation of the filled and empty minority band states. The magnetic sur-face anisotropy originates from the spin-orbit coupling of occupied and unoccupied states of the minority band. The dominant term in the MAE is, therefore, the spin-orbit sec-ond order perturbation term,
whereuandorepresent unoccupied and occupied spin-down states and is the spin-orbit coupling constant.38 When the coupling through Lzis stronger, the MAE becomes positive and the system presents perpendicular anisotropy.42 There-fore, the induction of magnetic anisotropy depends on of Co and on the actual states that have a probability of mixing; the smaller the difference in energy, the larger the MAE is. Within this scheme, the positive shift of MAE would be re-lated to the decreasing difference in the d orbital energy of the Co and the capping atom. Since these energy differences are −2.37, −1.44, and −0.21 eV for Cu, Ag, and Au, respec-tively, the trend of increasing MAE that is expected to follow is Co/Cu⬍Co/Ag⬍Co/Au. The same concepts may be ex-trapolated to the Co/Minterfaces at the polyhedron facets of the irregular Co particles. Therefore, one could expect an increasing surface anisotropy in those facets following the trend alumina, Cu, Ag, and Au capped.
Very enlightening in understanding the particle uniaxial anisotropy are the calculations of MAE for a Co cluster built by successively adding pairs of layers, with one at each side. Although the starting finite Co monolayer has planar aniso-tropy, just as an infinite monolayer Co thin film, the MAE decreases as facets grow from each side until it changes sign, i.e., the particle becomes uniaxial when two facets are added to the closed shell cluster.37This mechanism may be classi-fied as shape anisotropy. Superimposed to this mechanism is the interaction with the matrix which will add a positive shift to the MAE of the facets following the trends Co/alumina, Co/Cu, Co/Ag, and Co/Au and thus qualitatively explaining our observation. The fact that capping with Cu already in-creases Keffin our sample is relevant, since this implies that
the predominant anisotropy is always positive. Indeed, if the surface MAE of the Co/Al2O3 particle had been negative,
the capping with Cu would have implied a compensation of MAE and, consequently, a decrease inKeff, which is contrary to our experimental result. With respect to the Cu capping, our experimental result also seems to contradict the reduc-tion in MAE that was predicted in the calculareduc-tions for closed shell Co clusters with Cu additional facets or embedded in Cu.34,37
broadening of the out-of-plane d electron minority band while keeping the in-plane band unmodified. The effect is a net increase in mL⬜, while mL
remains constant. Conse-quently, the absolute value ofmLshould increase as well关Eq. 共2兲兴. Ultimately, this would translate into an increase inKS, after the simple but powerful relation proposed by Bruno43 that correlates the orbital moment anisotropy 共OMA兲 with the interface magnetocrystalline anisotropy energy共MAE兲,
whereis the Co spin-orbit coupling constant.
In a recent paper,44the limits of validity of this expression have been assessed in the case of a Co thin film with an interface of a different metal, in particular, Cu and Au. It is argued that Eq. 共8兲 is well fulfilled in the case of a Co/Cu interface since the s.o. coupling of Cu is low. In contrast, they find that Eq. 共8兲 may not hold in the case of a Co/Au interface since the Au s.o. coupling is large. However, no simple relationship between the MAE and OMA is given in that paper. At any rate, in the present work, we conjecture that Eq. 共8兲 holds for the four Co/Cu, Co/Ag, and Co/Au particle interfaces and check later for the consistency of the results for the Co/Cu and Co/Au cases.
In our experiment, the separation between mL
andmL⬜ is not possible. However, from Eq. 共2兲, one may obtain an ap-proximate relation between both parameters for the spherical particle approximation, namely,mL⬜=共3mL− 2mL
. For a non-spherical particle, the constants may differ but the linear de-pendence is maintained. Therefore, KS can be expressed in terms ofmLandmL
. One can considermL
to be identical to that of the bulk,mLbulk, since it is related to the Co-Co bond-ing within the Co surface atoms and their distances and in-teractions can be approximated to be those of the bulk. Sub-stituting in Eq.共8兲, one obtainsKS⬀共mL−mLbulk兲. The relative variation of KS for a given capping with respect to the Co/Al2O3 alumina-capped KS
, ⌬KS=KS−KS Al
can be ex-pressed as
KS Al =
where 共mLAl/mS兲surf is the averaged ratio of orbital moment with respect to the spin moment at the surface of the alumina-capped sample.
This relation holds under the assumption thatmSdoes not vary. In Fig. 11, the relative variation ofKS is plotted as a function of the relative variation of共mL/mS兲surf, both normal-ized to the values for Co/Al2O3. An increase in nearly a
factor of 2 in共mL/mS兲surf, when capping with Au, induces an increase inKS by nearly the same factor.
The correlation found is very satisfactory, as the relative variation of the two magnitudes proposed in Eq.共9兲is nearly followed. The difference in slope of the linear dependence may result from the rough approximation implied in the ap-plication of Eq. 共2兲, which is strictly valid for the spherical particle. At any rate, this result shows that the origin of the surface anisotropy is directly connected with the increase in 共mL/mS兲surf, which is in agreement with Bruno’s model.
Evidently, the quantitative agreement relies on the conjecture that mL
remains constant, irrespective of the capping ele-ment. This conjecture is based on the similar assumption successfully applied in the analysis of Co thin films capped with noble metals such as Cu or Au.22
In the present study, the conjecture of fulfillment of Bruno’s relation holds for the capped particles. This conclu-sion is in line with most previous work testing 关Eq. 共8兲兴. However, let us note that it is in contradiction with the pre-dicted and found decrease in perpendicular anisotropy in the Co/Au interface in a Co thin film sandwiched between Au films.44The different topologies of particle and film probably play a role in this difference.
The increase in induced mnd in Cu, Ag, and Au is prob-ably caused by the corresponding increased polarizability in that trend. The spin-orbit coupling of the noble metal seems to play a second order role in this mechanism. It gives rise to an extra component to the orbital momentmL
at the interfa-cial noble metal atom but is 2 orders of magnitude smaller than that of Co in the largest case, i.e., whenM= Au.
The emerging interaction scheme at the Co/Minterface is that, on one hand, the exchange polarized Co 3d band is antiferromagnetically coupled to the 4p band via intra-atomic spin-dependent hybridization and ferromagnetically coupled to the exchange split nd band of the M cap via 3d-ndhybridization, on the other. In the case of Cu capping, there is evidence of the Cu 3d polarized band to be antifer-romagnetically coupled to the 4p band via intra-atomic hy-bridization. Most probably, the 3d band of Co hybridizes with the 4p band of Cu, as proposed in Co/Cu thin films.10
In conclusion, the systematic increase inKSwith capping in the trends Cu, Ag, and Au has been correlated with the increase in the Co 3d meanmL, which is caused by hybrid-ization with the capping metal ndand共n+ 1兲pbands.
This work has been partly funded by Grants No. MAT05-1272 and No. MAT05-02454 from MEC, and PM-012,
IMANA, and CAMRADS from DGA. We thank Jesús González Casablanca for his valuable help with thin film preparation for TEM observation.
1F. Luis, J. M. Torres, L. M. García, J. Bartolomé, J. Stankiewicz,
F. Petroff, F. Fettar, J. L. Maurice, and A. Vaures, Phys. Rev. B 65, 094409共2002兲.
2R. Yanes, O. Chubykalo-Fesenko, H. Kachkachi, D. A. Garanin, R. Evans, and R. W. Chantrell, Phys. Rev. B 76, 064416共2007兲. 3P. Gambardella, S. Rusponi, M. Veronese, S. S. Dhesi, C. Grazioli, A. Dallmeyer, I. Cabria, R. Zeller, P. H. Dederichs, K. Kern, C. Carbona, and H. Brune, Science 300, 1130共2003兲. 4F. Bartolomé, F. Luis, F. Petroff, L. M. García, J. Bartolomé, V.
Cros, and H. Jaffres,J. Magn. Magn. Mater. 272-276, e1275 共2004兲.
5L. M. García, F. Bartolomé, J. Bartolomé, F. Luis, F. Petroff, C.
Deranlot, F. Wilhelm, A. Rogalev, P. Bencok, and N. B. Brookes, J. Magn. Magn. Mater. 316, e23共2007兲.
6F. Luis, J. Bartolomé, F. Bartolomé, M. J. Martinez, L. M.
García, F. Petroff, C. Deranlot, F. Wilhelm, and A. Rogalev, J. Appl. Phys. 99, 08G705共2006兲.
7F. Luis, F. Bartolomé, F. Petroff, J. Bartolomé, L. M. García, C.
Deranlot, H. Jaffrès, M. J. Martínez, P. Bencok, F. Wilhelm, A. Rogalev, and N. B. Brookes, Europhys. Lett. 76, 142共2006兲. 8D. Weller, Y. Wu, J. Stöhr, M. G. Samant, B. D. Hermsmeier,
and C. Chappert, Phys. Rev. B 49, 12888共1994兲.
9M. G. Samant, J. Stöhr, S. S. P. Parkin, G. A. Held, B. D.
Herms-meier, F. Herman, M. van Schilfgaarde, L.-C. Duda, D. C. Man-cini, N. Wassdahl, and R. Nakajima, Phys. Rev. Lett. 72, 1112 共1994兲.
10S. Pizzini, A. Fontaine, Ch. Giorgetti, E. Dartyge, J. F. Bobo, M.
Piecuch, and F. Baudelet, Phys. Rev. Lett. 74, 1470共1995兲. 11N. Jaouen, F. Wilhelm, A. Rogalev, J. M. Tonnerre, T. K. Johal,
and G. van der Laan, IEEE Trans. Magn. 41, 3334共2005兲; N. Jaouen, F. Wilhelm, A. Rogalev, J. Goulon, L. Ortega, J. M. Tonnerre, B. Rodmacq, and A. Yaresko, J. Phys.: Condens. Mat-ter 20, 095005共2008兲.
12F. Wilhelm, M. Angelakeris, N. Jaouen, P. Poulopoulos, E. Th.
Papaioannou, Ch. Mueller, P. Fumagalli, A. Rogalev, and N. K. Flevaris, Phys. Rev. B 69, 220404共R兲 共2004兲.
13J. Briático, J. L. Maurice, J. Carrey, D. Imhoff, F. Petroff, and A.
Vaures, Eur. Phys. J. D 9, 517共1999兲.
14J. L. Maurice, J. Briático, J. Carrey, F. Petroff, L. F. Schelp, and
A. Vaurès, Philos. Mag. A 79, 2921共1999兲.
15D. Babonneau, F. Petroff, J.-L. Maurice, F. Fettar, and A. Vaures,
Appl. Phys. Lett. 76, 2892共2000兲.
16T. Saito, T. Katayama, Y. Kurosaki, M. Endo, S. Saito, T.
Ka-mino, K. Kobayashi, Y. Suzuki, T. Nagahama, S. Yuasa, T. Koide, T. Shidara, H. Manaka, and H. Tokano, J. Magn. Magn. Mater. 272-276, e1489共2004兲.
17C. Morawe and H. Zabel, J. Appl. Phys. 77, 1969共1995兲. 18O. Kitakami, H. Sato, Y. Shimada, F. Sato, and M. Tanaka, Phys.
Rev. B 56, 13849共1997兲.
19J. Bartolomé, F. Bartolomé, L. M. García, F. Luis, F. Petroff, V.
Cros, H. Jaffrès, and A. Vaurès, inSmart Materials for Ranging Systems, ARW NATO No. 4 edited by J. Franse, V. Eremenko, and V. Sirenko共Springer, 2006兲, p. 1.
20P. Carra, B. T. Thole, M. Altarelli, and X. Wang, Phys. Rev. Lett.
21B. T. Thole, P. Carra, F. Sette, and G. van der Laan, Phys. Rev.
Lett. 68, 1943共1992兲.
22J. Stöhr, J. Electron Spectrosc. Relat. Phenom. 75, 253共1995兲. 23J. P. Rueff, R. M. Galera, C. Giorgetti, E. Dartyge, C. Brouder,
and M. Alouani, Phys. Rev. B 58, 12271共1998兲.
24J. M. Torres, F. Luis, L. M. García, J. Bartolomé, J. Stankiewicz, F. Petroff, F. Fettar, and A. Vaurés, J. Magn. Magn. Mater. 242-245, 575共2002兲.
25C. T. Chen, Y. U. Idzerda, H.-J. Lin, N. V. Smith, G. Meigs, E.
Chaban, G. H. Ho, E. Pellegrin, and F. Sette, Phys. Rev. Lett. 75, 152共1995兲.
26W. A. Sucksmith and J. E. Thompson, Proc. R. Soc. London, Ser.
A 225, 362共1954兲.
27M. Tischer, O. Hjorstam, D. Arvanitis, J. H. Dunn, F. May, K.
Baberschke, J. Trygg, J. M. Wills, B. Johansson, and O. Eriks-son, Phys. Rev. Lett. 75, 1602共1995兲.
28T. Koide, H. Miyauchi, J. Okamoto, T. Shidara, A. Fujimori, H.
Fukutani, K. Amemiya, H. Takeshita, S. Yuasa, T. Katayama, and Y. Suzuki, Phys. Rev. Lett. 87, 257201共2001兲.
29N. Nakajima, T. Koide, T. Shidara, H. Miyauchi, H. Fukutani, A.
Fujimori, K. Iio, T. Katayama, M. Nývlt, and Y. Suzuki, Phys. Rev. Lett. 81, 5229共1998兲.
30D. A. Eastham and J. W. Kirkman, J. Phys.: Condens. Matter 12,
31H. A. Dürr, S. S. Dhesi, E. Dudzik, D. Knabben, G. van der
Laan, J. B. Goedkoop, and F. U. Hillebrecht, Phys. Rev. B 59, R701共1999兲.
32B. T. Thole and G. van der Laan, Phys. Rev. A 38, 1943共1988兲. 33A. García Prieto, M. L. Fdez-Gubieda, J. Chaboy, M. A.
Laguna-Marco, T. Muro, and T. Nakamura, Phys. Rev. B 72, 212403 共2005兲.
34Y. Xie and J. A. Blackman, Phys. Rev. B 66, 155417共2002兲. 35A. N. Mansour, J. W. Cook, Jr., and D. E. Sayers, J. Phys. Chem.
36M. Vijayakumar and M. S. Gopinathan, J. Mol. Struct.:
THEOCHEM 361, 15共1996兲.
37Y. Xie, and J. Blackman, J. Phys.: Condens. Matter 16, 3163 共2004兲.
38D. S. Wang, R. Wu, and A. J. Freeman, J. Magn. Magn. Mater.
39R. Wu and A. J. Freeman, J. Magn. Magn. Mater. 200, 498 共1999兲.
40B. Újfalussy, L. Szunyogh, P. Bruno, and P. Weinberger, Phys.
Rev. Lett. 77, 1805共1996兲.
41L. Szunyogh, B. Újfalussy, U. Pustogowa, and P. Weinberger,
Phys. Rev. B 57, 8838共1998兲.
42J. Stöhr, J. Magn. Magn. Mater. 200, 470共1999兲. 43P. Bruno, Phys. Rev. B 39, 865共1989兲.
44C. Andersson, B. Sanyal, O. Eriksson, L. Nordström, O. Karis,